Heteroepitaxial growth of TiN film on MgO (100) by reactive magnetron sputtering
© Chen et al.; licensee Springer. 2014
Received: 25 June 2014
Accepted: 10 September 2014
Published: 3 October 2014
TiN thin films were deposited on MgO (100) substrates at different substrate temperatures using rf sputtering with Ar/N2 ratio of about 10. At 700°C, the growth rate of TiN was approximately 0.05 μm/h. The structural and electrical properties of TiN thin films were characterized with x-ray diffraction (XRD), atomic force microscopy (AFM), scanning electron microscopy (SEM), transmission electron microscopy (TEM), and Hall measurements. For all deposition conditions, XRD results show that the TiN films can be in an epitaxy with MgO with cube-on-cube orientation relationship of (001)TiN // (001)MgO and TiN // MgO. TEM with selected-area electron diffraction pattern verifies the epitaxial growth of the TiN films on MgO. SEM and AFM show that the surface of the TiN film is very smooth with roughness approximately 0.26 nm. The minimum resistivity of the films can be as low as 45 μΩ cm.
KeywordsHeteroepitaxial TiN MgO (100) High quality rf sputtering
Titanium nitride (TiN) thin films have been extensively used in a wide range of applications as wear-protective coatings on mechanical components, cutting tools, decorations, as well as diffusion barriers and metal gates in integrated circuits [1, 2], owing to its remarkable physical and chemical properties such as high hardness, high thermal stability, low electrical resistivity, and high wear excellent corrosion resistance [3, 4]. Also, Pure TiN films are highly reflective and gold in color and have found applications in jewelery and optics . Studies on TiN properties have solved significant problems, such as the reduction of the usefulness of TiN films for corrosion-resistant coatings and for diffusion barriers in the films . Grigorov et al. reported that TiN has uses in microelectronics due to its efficiency in preventing aluminum diffusion into silicon in Al-TiN-Si trilayers at up to 550°C .
In order to deposit thin films of TiN on various substrates, it is common to use processes such as physical vapor deposition (PVD) , chemical vapor deposition (CVD) , atomic layer deposition (ALD) , and hallow cathode ionic plating (HCIP). Among those processes, the PVD process is known to be easy and to present a good adhesion between the film and the substrates of metals and ceramics . Among various PVD processes, dc reactive sputtering is commonly used for deposition of polycrystalline and single-crystalline films. For epitaxial growth, TiN films have been often grown on an MgO substrate based on a consideration of the same rock salt structure and small lattice mismatch (<1% at room temperature) between their lattice parameters . Previous studies of TiN deposition on the MgO (100) substrate showed that high-quality epitaxial TiN films can be obtained using ultrahigh vacuum dc reactive magnetron sputtering of pure Ti [13–16]. Reactive radio-frequency (rf) magnetron sputtering of a Ti target has been demonstrated for deposition of TiN polycrystalline films with preferred orientation dependence on argon/nitrogen ratio and substrate temperature . In addition, Ingason et al. indicated that a minimum substrate temperature of 200°C is required for a good epitaxy. Also, substrate temperatures of 100°C and below yield low density, polycrystalline films with in-plane texture of ±12° around the main crystal axis of the MgO substrate .
In this article, we report heteroepitaxial growth of TiN deposited on MgO (100) using rf reactive magnetron sputtering in high vacuum at 600°C and 700°C. The crystallinity, surface morphologies, and microstructure of deposited films were characterized by x-ray diffraction (XRD), transmission electron microscopy (TEM), scanning electron microscopy (SEM), and atomic force microscopy (AFM).
In our previous study of rf reactive sputtering of a Ti target for TiN polycrystalline films on Si (100), we found an optimum condition for growth of <100 > preferentially oriented TiN films  which was used for the present study for epitaxial growth of TiN films on MgO (100). TiN epilayers were deposited on the MgO (100) substrate using a 13.56 MHz rf sputtering apparatus without a bias voltage. MgO (100) of 2-in size was chosen as a substrate. The vacuum chamber was equipped with a cryopump to reduce the pressure to about approximately 1 × 10-6 Torr. An elemental Ti target (99.99% purity) was reactively sputtered in a mixture of Ar (99.999%) and pure N2 (99.9999%) with a ratio of 10:1, and the total gas pressure during the growth was 1 mTorr. The distance between the substrate holder and the target was 20 cm. The rf power was 200 W. MgO substrates were ultrasonically cleaned in acetone and ethanol and dried with dry N2 and immediately inserted into the vacuum chamber. Prior to TiN growth, the MgO (100) substrate was heat-treated in a vacuum of 5 × 10-6 torr at 700°C for 2 h, and the target was sputtered to clean the surface for 10 min with a shutter covering the substrate. Final, TiN epilayers were prepared on the MgO substrate at 600°C and 700°C. The epitaxial nature of the TiN (200) layer was examined using x-ray diffraction in ω-2θ, rocking curve (Siemens D5000, Siemens, Shinagawa-ku, Japan), and ø-scan mode with CuKα radiation (Bruker D8, Bruker Optik GmbH, Ettlingen, Germany). Surface morphology and microstrucure of deposited TiN in a cross section were analyzed in a field emission SEM (FE-SEM; Hitachi S-4300, Hitachi, Ltd, Chiyoda-ku, Japan) and TEM (Philips Tecnai 20, Philips, Amsterdam, The Netherlands). The cross-sectional TEM specimens were prepared by focused ion beam technique. The morphology of the film with surface roughness was investigated by AFM. Room-temperature electrical resistivities were determined with a four-point probe (Keithley 237, Keithley Instruments, Inc., Minato-ku, Japan).
Results and discussion
Resistivity measurements can be used to qualitatively determine the defect concentration in a metal film. Also, the resistivity of TiN films depends on microstructure, preferred orientation, and stoichiometry. TiN films exhibit resistivity of 45 μΩ cm in average at room temperature higher than the bulk crystal value of 13 μΩ cm. The result is in agreement with the reports of Yokota et al.  and Biunno et al. . In contrast, polycrystalline TiN films deposited on Si (100) in the same sputtering condition have the resistivities in the range of 200 μΩ cm, implying that grain boundaries have strong effects on electron scattering.
Compared to other studies on electrical resistivity of TiN, the value is very close to present accepted values. Therefore, the result implies that the film quality is reasonably good.
In summary, high-quality epitaxial TiN (100) films can be deposited on a 2-in MgO (100) substrate at 700°C by rf reactive sputtering process in a high vacuum. Structural characterization shows that epitaxial TiN films exhibit a smooth surface and a coherent good interface with MgO. Also, TiN films of 100-nm thickness are close to stoichiometry and strain-relaxed.
This work was supported by the National Science Council (NSC) of Taiwan under contract no. NSC 103-2622-E-492-010-CC3.
- Sundgren JE: Structure and properties of TiN coatings. Thin Solid Films 1985, 128: 21–44. 10.1016/0040-6090(85)90333-5View ArticleGoogle Scholar
- Kothari DC, Scardi P, Gialanella S, Guzman L: Structural analysis of TiNx films prepared by reactive-ion-beam-enhanced deposition. Philos Mag B 1990, 61: 627–637. 10.1080/13642819008219298View ArticleGoogle Scholar
- Hogmark S, Jacobson S, Larsson M: Design and evaluation of tribological coatings. Wear 2000, 246: 20–33. 10.1016/S0043-1648(00)00505-6View ArticleGoogle Scholar
- Cunha L, Ansritschky M, Rebouta L, Pischow K: Corrosion of CrN and TiAlN coatings in chloride-containing atmospheres. Surf Coat Technol 1999, 116–119: 1152–1160.View ArticleGoogle Scholar
- Perry AJ, Georgson M, Sproul WD: Variations in the reflectance of TiN, ZrN and HfN. Thin Solid Films 1988, 157: 255–265. 10.1016/0040-6090(88)90007-7View ArticleGoogle Scholar
- Hinode K, Homma Y, Horiuchi M, Takahashi T: Morphology-dependent oxidation behavior of reactively sputtered titanium–nitride films. J Vac Sci Technol A 1997, 15: 2017–2022. 10.1116/1.580673View ArticleGoogle Scholar
- Grigorov GI, Grigorov KG, Stayanova M, Vignes JL, Langeron JP, Denjean P: Aluminium diffusion in titanium nitride films. Efficiency of TiN barrier layers. Appl Phys A 1993, 57: 195–197. 10.1007/BF00331444View ArticleGoogle Scholar
- Jun K, Shimogaki Y: Effect of partial pressure of TiCl4 and NH3 on chemical vapor deposition titanium nitride (CVD-TiN) film Cl content and electrical resistivity. Jpn J Appl Phys 2004, 43: L519-L521. 10.1143/JJAP.43.L519View ArticleGoogle Scholar
- Paranjpe A, IslamRaja M: Chemical vapor deposition TiN process for contact/via barrier applications. J Vac Sci Technol B 1995, 13: 2105–2114.View ArticleGoogle Scholar
- Kim J, Hong H, Ghosh S, Oh KY, Lee C: Physical properties of highly conformal TiN thin films grown by atomic layer deposition. Jpn J Appl Phys 2003, 42: 1375–1379. 10.1143/JJAP.42.1375View ArticleGoogle Scholar
- Li Y, Qui L, Wang F: The electrochemical corrosion behavior of TiN and (Ti, Al) N coatings in acid and salt solution. Corros Sci 2003, 45: 1367–1381. 10.1016/S0010-938X(02)00223-8View ArticleGoogle Scholar
- Karr BW, Petrov I, Cahill DG, Greene JE: Morphology of epitaxial TiN (001) grown by magnetron sputtering. Appl Phys Lett 1997, 70: 1703–1705. 10.1063/1.118675View ArticleGoogle Scholar
- Kawakubo T, Sano K, Oose M: Heteroepitaxial TiN films grown by reactive ion beam epitaxy at room temperature. Jpn J Appl Phys 1993, 32: L1692-L1694. 10.1143/JJAP.32.L1692View ArticleGoogle Scholar
- Lawanda NS, Frencha PJ, Briaireb JJ, Frijns JHM: Thin Titanium Nitride films deposited using DC magnetron sputtering used for neural stimulation and sensing purposes. Procedia Eng 2012, 47: 726–729.View ArticleGoogle Scholar
- Ljungcrantz H, Odén M, Hultman L, Greene JE, Sundgren JE: Nanoindentation studies of single‒crystal (001)‒, (011)‒, and (111)‒oriented TiN layers on MgO. J Appl Phys 1996, 80: 6725–6733. 10.1063/1.363799View ArticleGoogle Scholar
- Shin CS, Rudenja S, Gall D, Hellgren N, Lee TY, Petrov I, Greene JE: Growth, surface morphology, and electrical resistivity of fully strained substoichiometric epitaxial layers on MgO (001). J Appl Phys 2004, 95: 356–362. 10.1063/1.1629155View ArticleGoogle Scholar
- Li TQ, Noda S, Tsuji Y, Ohsawa T, Komiyama H: Initial growth and texture formation during reactive magnetron sputtering of TiN on Si (111). J Vac Sci Technol A 2002, 20: 583–588. 10.1116/1.1458944View ArticleGoogle Scholar
- Ingason AS, Magnus F, Olafsson S, Gudmundsson JT: Morphology of TiN thin films grown on MgO (001) by reactive dc magnetron sputtering. J Vac Sci Technol A 2010, 28: 912–915.View ArticleGoogle Scholar
- Chen WC, Wang WL, Tiwari RN, Chang L: Growth and characterization of diamond films on TiN/Si (100) by microwave plasma chemical vapor deposition. Diamond Relat Mater 2009, 18: 124–127. 10.1016/j.diamond.2008.10.018View ArticleGoogle Scholar
- Pryds N, Cockburn D, Rodrigo K, Rasmussen IL, Knudesn J, Schou J: Growth of thin films of TiN on MgO (100) monitored by high-pressure RHEED. Appl Phys A 2008, 93: 705–710. 10.1007/s00339-008-4700-2View ArticleGoogle Scholar
- Yokota K, Nakamura K, Kasuya T, Mukai K, Ohnishi M: Resistivities of titanium nitride films prepared onto silicon by an ion beam assisted deposition method. J Phys D Appl Phys 2004, 37: 1095–1101. 10.1088/0022-3727/37/7/023View ArticleGoogle Scholar
- Biunno N, Narayan J, Srivatsa AR, Holland OW: Laser deposition of epitaxial titanium nitride films on (100) MgO. Appl Phys Lett 1989, 55: 405–407. 10.1063/1.101881View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.